Tuning Electrical Properties in Amorphous Zinc Tin Oxide Thin Films for Solution Processed Electronics R. Devi Chandra,†,# Manohar Rao,†,# Keke Zhang,† Rajiv Ramanujam Prabhakar,† Chen Shi,‡ Jie Zhang,⊥ Subodh G. Mhaisalkar,†,§,⊥ and Nripan Mathews*,†,§,¶ †
Energy Research Institute, Nanyang Technological University, Singapore 637553 School of Physical and Mathematical Sciences, Nanyang Technological University, Singapore 637371 § School of Materials Science and Engineering, Nanyang Technological University, Singapore 637553 ⊥ Institute of Materials Research and Engineering, 3 Research Link, Singapore 117602 ¶ Singapore-Berkeley Research Initiative for Sustainable Energy (SinBeRISE), 1 Create Way, Singapore 138602 ‡
S Supporting Information *
ABSTRACT: Solution processed zinc tin oxide (ZTO) thin ﬁlm transistors (TFTs) were fabricated by varying the Zn/Sn composition. The addition of Sn to the zinc oxide (ZnO) ﬁlms resulted in improved electrical characteristics, with devices of Zn0.7Sn0.3O composition showing the highest mobility of 7.7 cm2/(V s). An improvement in subthreshold swings was also observed, indicative of a reduction of the interfacial trap densities. Mobility studies at low temperature have been carried out, which indicated that the activation energy was reduced with Sn incorporation. Kelvin probe force microscopy was performed on the ﬁlms to evaluate work function and correlated to the metal−semiconductor barrier indicating Zn0.7Sn0.3O ﬁlms had the smallest barrier for charge injection. Organic−inorganic hybrid complementary inverters with a maximum gain of 10 were fabricated by integrating ZTO TFTs with poly-3-hexylthiophene (P3HT) transistors. KEYWORDS: zinc tin oxide, amorphous semiconductors, thin ﬁlm transistors, CMOS inverter, Kelvin probe, solution processing
mobility and trap density, and its inﬂuence on the device performance is examined in detail. Low temperature charge transport studies have been carried out, and the eﬀect of varying composition on the activation energy has been studied. In addition, we carried out Kelvin probe force microscopy (KPFM) studies on such ﬁlms to evaluate the change of surface potential induced by composition change in ZTO. Optimized ZTO TFTs were combined with p-type transistors fabricated from poly-3-hexylthiophene (P3HT) to form hysteresis free complementary inverters with high gain.
Synthesis of ZTO Films. The ZTO solution was prepared by mixing ZnCl2 and SnCl2 precursors in acetonitrile at diﬀerent molar ratios; 0.136g of ZnCl2 and 0.189g of SnCl2 were added to 10 mL of acetonitrile solution each to make stock solution of the metal salt precursors. In order to improve the solubility of the salt precursor, 500 μL of acetic acid was added to the ﬁnal precursor solution. The molar ratios of (Zn/Sn) in the ﬁnal precursor solutions were varied as 1:0, 0.7:0.3, 0.5:0.5, and 0.3:0.7. The solution was stirred at 60 °C in air for 12 h and ﬁltered using 0.2 μm ﬁlters. The stock solutions were stable and expressed no precipitation during weeks of usage. Film Characterization. To conﬁrm the chemical composition of the various ﬁlms, X-ray photoelectron spectroscopy (XPS) measurements were carried out with a monochromatic X-ray source (Specs Received: March 19, 2013 Accepted: December 11, 2013
Figure 1. (a) Survey scan for ZnO and ZTO ﬁlms highlighting the Zn 2p, Sn 3p, O 1s, and Sn 3d orbitals. (b) Narrow scan for Zn 2p. (c) Narrow Scan for Sn 3d. (d) Narrow scan for O 1s.
Focus 500 and Omicron EA125) at Al Kα (1486.7 eV) under ultrahigh vacuum (UHV) condition at room temperature. Surface potential measurements (KPFM) were carried out on a commercial Asylum Research MF3PD system, using a platinum-coated silicon cantilever (Olympus Model AC240 TM, resonant frequency of 70 kHz, spring constant of 2 N/m, tip height = 14 μm, and tip radius ≈ 30 nm). Topographic noncontact imaging was performed in frequency modulation mode, while KPFM data was recorded simultaneously in amplitude modulation mode. The surface potential was evaluated in order to extract the Fermi level of the ﬁlms modiﬁed due to the composition changes introduced by the varying Sn concentration in ZTO ﬁlms. Device Fabrication. ZTO TFTs were fabricated by spin coating the solution on precleaned commercial 200 nm Si3N4 ﬁlms on silicon (p-type,  oriented) substrate. The precursor solution was spin coated at 4000 rpm for 30 s resulting in a ﬁlm thickness of ∼15 nm measured using atomic force microscopy. The ﬁlms were then annealed at 500° C for 1 h in air, and aluminum was deposited as top electrodes forming transistors of various channel lengths and channel width. Typical dimensions were 1000 μm as channel width and 100 μm as the channel length. Following the formation of the Zn0.7Sn0.3O layer, the inverters were completed by spin coating P3HT (10 mg/mL, dichlorobenzene) on hexamethyldisilazane (HMDS) treated dielectric substrate. Gold as the source-drain electrode was thermally evaporated on both P3HT and ZTO device to give a channel length of 100 μm and channel width of 1000 μm. Electrical Characterization. Transistor measurements were carried out in both air and vacuum using a Keithley 4200 semiconductor analyzer. No appreciable diﬀerences in the performance of the ZTO transistors were noted when measuring the devices in both conditions. Measurements of temperature dependent mobility of various Zn/Sn ratio TFT samples were conducted in the cryogenic probe station (Lakeshore-1200). To ensure performance uniformity, TFT data presented here are reported from 10 devices fabricated for each molar concentration.
RESULTS AND DISCUSSION
Physical Characteristics. The spun coated and annealed ﬁlms were ﬁrst analyzed using XPS to conﬁrm the composition. Figure 1a shows the survey scans of the various prepared samples. The Zn 2p3/2 and the Sn 3d5/2 located at 1022.7 and 487.5 eV, respectively, were monitored to estimate the relative composition of the ﬁlms. They were in line with the nominal compositions of the precursor solutions. Since Sn can exist in its Sn2+ or Sn4+ oxidation state (which can result in p-type SnO or n-type SnO2), the oxidation states of samples prepared from SnCl2 solutions were examined. The narrow scan for Sn 3d and O1s is shown in the Figure 1c,d. The 3d5/2 shows only one component at 487.5 eV ruling out the coexistence of SnO and SnO2.15,16 Since the binding energy of Sn in SnO2 (486.3− 487.1 eV) is reported to be only slightly higher than Sn in SnO (485.8−486.9 eV), the binding energy of Sn alone is not suﬃcient to distinguish the chemical states of the Sn sample.17 The examination of the O1s spectrum reveals two components located at 531.5 and 532.7 eV with the higher binding energy component attributable to adsorbed hydroxyls. The atomic ratio (Sn/O) of 1:1.63 computed from Sn 3d and O1s peaks (taking into consideration atomic sensitivity factors) implies that the sample is oxygen-deﬁcient SnO2.17 In addition to the composition, the morphology of the samples was also examined, ZnO displayed a granular morphology with an average rms surface roughness of ∼6.8 nm, while the ZTO samples showed a smooth amorphous morphology with average surface roughness of 0.5 nm. The diﬀerence in the surface roughness may be attributed to the ZnO ﬁlms being polycrystalline while the ZTO samples are amorphous (Supporting Information).4 B
Figure 2. (a) Transistor I−V characteristics for pristine ZnO and Zn0.7Sn0.3O ratio devices with W/L 1000 μm/105 μm. (b) Transconductance response for varying Zn/Sn ratio FET fabricated on silicon nitride dielectric (inset) device architecture.
Figure 3. (a) Mobility and trap density extracted from the FET response plotted for devices with diﬀerent concentrations. (b) Plot of ln μ vs 1000/T for Zn/Sn molar ratio samples measured at VG of 10 V. (Inset) Work-function diﬀerence between Al electrode and the material measured using KPFM.
Electrical Characteristics. ZTO TFTs fabricated with diﬀerent molar concentration with Al source drain electrodes showed n-channel transport. The saturation regime mobility (μ) and threshold voltage (VTH) parameters were extracted using the standard expression, Ids =
WμC i (VG − VTH)2 L
high conductivity indicative of high carrier density induced by oxygen vacancies. For higher Sn concentrations in ZnxSn1−xO, there was a slight reduction in mobility as indicated in Figure 3a. The subthreshold swing decreases with Sn content (Supporting Information), indicating that the extremely low mobility and low subthreshold slope in ZnO TFTs can be attributed to low carrier concentration and high density of surface states at the interface between the channel and gate dielectric. In particular, the grains as seen using atomic micrograph images for ZnO ﬁlms may induce a signiﬁcant number of interfacial states resulting in lower ﬁeld eﬀect mobility. Figure 3a shows the plot of trap density extracted for various Zn/Sn molar ratio ﬁlms using the equation
where μ is mobility, W and L is the channel length and width, Ci is gate dielectric areal capacitance, VG is the gate voltage, and VTH is the threshold voltage. Figure 2a compares the I−V characteristics of pristine ZnO TFTs against Zn0.7Sn0.3O TFTs, indicating an increase in saturation current for the same applied VG. The addition of Sn to the ZnO ﬁlms resulted in improved electrical characteristics, with devices of Zn0.7Sn0.3O ratio showing the highest mobility of 7.7 cm2/(V s). The other two ratios studied yielded mobilities of 5.4 cm2/(V s) (Zn0.5Sn0.5O) and 1.8 cm2/(V s) (Zn0.3Sn0.7O), respectively. Figure 2b displays a set of representative transfer characteristics for ZnxSn1‑xO transistors of diﬀerent Zn/Sn ratios. The mobility for all the devices was extracted from the transconductance curve at Vds of 40 V. The pure ZnO TFT prepared from ZnCl2 precursor shows nominal transistor characteristics with μ ∼ 10‑3 cm2/(V s) and on/oﬀ ratio of 103. The pure SnO2 ﬁlm, which did not show any gate voltage dependence, showed
max Ntrap =
⎞ C i ⎛ qs.s log e − 1⎟ ⎜ q ⎝ kBT ⎠
where kB is the Boltzmann constant, T is the temperature, e is the base of natural logarithm, q is the electronic charge, s.s is the reciprocal of subthreshold slope, and Ci is the areal dielectric capacitance. The maximum trap density was extracted for ZnO TFT with a reduction in trap density with increasing Sn concentration in the ﬁlm. On addition of Sn, the trap density reduces nearly by 2 orders of magnitude, going from 1.6 × 1018 cm−3 (ZnO) to 7.9 × 1016 cm−3 for Zn0.3Sn0.7O. C
Figure 4. (a) The switching characteristics of an inverter fabricated from p-channel P3HT and n channel Zn0.7Sn0.3O measured at various Vdd. (b) Corresponding gain for the inverter measured at diﬀerent Vdd. (Inset) Shows the circuit conﬁguration.
to Sn addition) could be the reason why ZTO ﬁlms of (0.7:0.3) composition have the best performance. These general trends still hold true for samples fabricated at ﬁner concentration intervals with samples lower than 30% Sn concentrations not resulting in high mobility devices (Figure S3, Supporting Information). Although the fabrication procedures utilized for fabricating these amorphous thin ﬁlms requires a rather high annealing temperature of 500 °C (incompatible with plastic substrates), the trends in the mobility values, as well as trap densities extracted here, should be applicable to ﬁlms formed through low temperature recipes such as combustion synthesis.21 On the basis of the optimized performance for Zn0.7Sn0.3O TFT, complementary inverters were fabricated using P3HTZTO TFTs. The schematic representation of the electrical connections is shown in the inset of Figure 4b. In the circuit, the input voltage Vin was applied to the common gate for both transistors. Plots of the output voltage Vout as a function of Vin under the diﬀerent supply voltages Vdd are shown in Figure 4a. No hysteresis was observed during the inverter action, reﬂecting excellent threshold voltage stability in devices. The measured voltage gain −dVout/dVin, an important parameter for subsequent stage switching, was of the order of ∼10 and 3 at Vdd of 40 V and Vdd of 15 V. As expected, the gain and switching point increases with applied Vdd.22 From the inverter output characteristics at Vdd = 40 V, an input high voltage (VIH) of 8.5 V and input low voltage (VIL) of 9.8 V could be measured at unity gain. Similarly, the devices have high and low output voltages of 12.7 and 7.8 V, which gives a low noise margin (MLN) of 1.8 V and high noise margin (MHN) of 4.2 V.
The eﬀect of varying Zn/Sn concentration on charge transport was studied by extracting activation energy of these devices by measuring the performance at variable temperatures. Figure 3b shows the plot of mobility measured at saturation gate voltages measured as a function of temperature. From the plot of ln μeff vs 1000/T the activation energy Ea was estimated using the equation, Ea = (−1000kB)((∂(ln μ)/(∂(1000/ T)))where kB is the Boltzmann constant and T is the temperature. All the devices showed thermally activated transport, with varying activation energy for diﬀerent Zn/Sn ratio samples. Figure 3b shows the dependence of activation energy of Zn/Sn ﬁlms measured at Vg of 10 V with Zn0.7Sn0.3O ﬁlms composition showing an activation energy of 90.4 meV while it reduces to ∼40−50 meV at higher Sn concentrations. This reduction in activation energy could be connected to the lower trap densities extracted previously. Although the mobility values for all the ZTO devices show performance >1 cm2/(V s), it is surprising that the composition which yielded the highest mobility also had the highest activation energy for electron transport. In order to investigate the possibility of injection barriers at the metal electrode−semiconductor interface aﬀecting the performance of the devices, KPFM measurements were performed. Surface potential of the samples were measured using KPFM by initially heating the active device at 100° C for 15 min in order to eliminate the eﬀect of adsorbed moisture on the samples. The samples showed a distinct variation of surface potential as a function of Sn composition in ZnO ﬁlms. The incorporation of Sn atoms to ZnO matrix resulted in an increase of the surface potential. The KPFM measurements have been used to evaluate the surface potential of ZTO ﬁlms, which is indicative of work function of the sample, based on the equation ΔSP = (φtip − φs)/e, where φtip is the work function of the tip (Pt coated on Si) and φs is that of the sample. The aluminum electrode (ϕm = 4.2 eV) used as the source-drain electrode of the ZTO FETs is used as an internal reference directly on each sample. The diﬀerence in the work function of Al and ZTO ﬁlm has been used to calculate the injection barrier for each of the samples.18−20 The work-function diﬀerence (ϕms) between the Al electrodes and the KPFM measured work-function of ZTO is plotted in the inset of Figure 3b. The addition of Sn resulted in an increased barrier for electron injection with Zn0.7Sn0.3O ﬁlms showing the lowest barrier. This low injection barrier coupled with lower trap density (due
CONCLUSION In summary, the eﬀect on Zn/Sn composition change on the electrical characteristics was studied by fabricating solution processed ZTO FETs. The Zn/Sn composition ratio clearly has an eﬀect on ﬁlm morphology, electrical property, and surface potential. The addition of Sn concentration causes a signiﬁcant improvement of FET performance with a maximum mobility of 7.7 cm2/(V s). The increased Sn concentration is accompanied by a reduction in the trap densities within these devices as well as a modulation of the injection barrier at the metal− semiconductor junction. Reduced trap densities as well as low injection barrier between the electrode and ZTO ﬁlms D
(19) Khaderbad, M. A.; Tjoa, V.; Rao, M.; Phandripande, R.; Madhu, S.; Wei, J.; Ravikanth, M.; Mathews, N.; Mhaisalkar, S. G.; Rao, V. R. ACS Appl. Mater. Interfaces 2012, 4, 1434−1439. (20) Liscio, A.; Veronese, G.P.; Treossi, E.; Suriano, F.; Rossella, F.; Bellani, V.; Rizzoli, R.; Samori, P.; Palermo, V. J. Mater. Chem. 2011, 21, 2921−2931. (21) Kim, M. G.; Kanatzidis, M. G.; Facchetti, A.; Marks, T. J. Nat. Mat. 2011, 10, 382−388. (22) Tan, H. S.; Wang, B. C.; Kamath, S.; Chua, J.; Shojaei-Baghini, M.; Rao, V. R.; Mathews, N.; Mhaisalkar, S. G. IEEE Electron Device Lett. 2010, 31, 1311−1313.
determine the composition with the highest performance. Complementary inverters were fabricated, utilizing the optimized n-type ZTO composition along with p-type P3HT ﬁlms. This work demonstrates the potential of optimized ZTO FETs fabricated through a solution processed approach.
S Supporting Information *
Subthreshold swing values as well as atomic force microscopy measurements on the thin ﬁlms. This information is available free of charge via the Internet at http://pubs.acs.org/
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS The project was supported by A*STAR, Project No: 102 170 0318, and NRF-CREATE funding under the SinBeRISE program.
(1) Nomura, K.; Ohta, H.; Takagi, A.; Kamiya, T.; Hirano, M.; Hosono, H. Nature 2004, 432, 488−492. (2) Park, J. S.; Maeng, W. J.; Kim, H.S.; Park, J. S. Thin Solid Films 2012, 520, 1679−1693. (3) Banger, K. K.; Yamashita, Y.; Mori, K.; Peterson, R. L.; Leedham, T.; Richard, J.; Sirringhaus, H. Nat. Mater. 2011, 10, 45−50. (4) Oo, T. Z.; Devi Chandra, R.; Yantara, N.; Prabhakar, R. R.; Wong, L. H.; Mathews, N.; Mhaisalkar, S. G. Org. Electron. 2012, 13, 870−874. (5) Pal, B. N.; Dhar, B. M.; See, K. C.; Katz, H. E. Nat. Mater. 2009, 8, 898−903. (6) Lee, D. H.; Han, S. Y.; Herman, G. S.; Chang, C.H. J. Mater. Chem. 2009, 19, 3135−3137. (7) Park, K. B.; Seon, J. B.; Kim, G. H.; Yang, M.; Koo, B.; Kim, H. J.; Ryu, M. W.; Lee, S.Y. IEEE Electron Device Lett. 2010, 31, 311−313. (8) Kim, H. G.; Ahn, B. D.; Shin, H. S.; Jeong, W.H.; Kim, H.J. Appl. Phys. Lett. 2009, 94, 233501−233503. (9) Ryu, M. K.; Yang, S.; Park, S. H.; Hwang, C.-S.; Jeong, J.K. Appl. Phys. Lett. 2009, 95, 173508−173510. (10) Lee, C. G.; Dodabalapur, A. Appl. Phys. Lett. 2010, 96, 243501− 243503. (11) Nomura, K.; Ohta, H.; Takagi, A.; Kamiya, T.; Hirano, M.; Hosono, H. Nature 2004, 432, 488−492. (12) Nomura, K.; Ohta, H.; Ueda, K.; Kamiya, T.; Hirano, M.; Hosono, H. Science 2003, 300, 1269−1272. (13) Minami, T.; Takata, S.; Sato, H.; Sonohara, H. J. Vac. Sci. Technol. 1995, A13, 1095−1099. (14) Young, D. L.; Moutinho, H.; Yan, Y.; Coutts, T. J. J. Appl. Phys. 2002, 92, 310−319. (15) Hwang, S.; Kim, Y. Y.; Lee, J. H.; Seo, D. K.; Lee, J. Y.; Cho, H. K. J. Am. Ceram. Soc. 2012, 95, 324−327. (16) Kövér, L.; Kovács, Zs.; Sanjinés, R.; Moretti, G.; Cserny, I.; Margaritondo, G.; Pálinkás, J.; Adachi, H. Surf. Interface Anal. 1995, 23, 461−466. (17) Choi, W. K.; Sung, H.; Kim, K. H.; Cho, J. S.; Choi, S. C.; Jung, H.-J.; Koh, S. K.; Lee, C. M.; Jeong, K. J. Mater. Sci. Lett. 1997, 16, 1551−1554. (18) Bürgi, L.; Richards, T. J.; Friend, R. H.; Sirringhaus, H. J. Appl. Phys. 2003, 94, 6129−6137. E
This study examined the structural, chemical, and electrical properties of solution-processed (Zn,Sn)O3 (ZTO) films with various Sn/[Zn+Sn] ratios for potential applications to large-area flat panel displays. ZTO films with a Zn-rich composition had
Solution-processed gate dielectrics were fabricated with the combined ZrO2 and Al2O3 (ZAO) in the form of mixed and stacked types for oxide thin film transistors (TFTs). ZAO thin films prepared with double coatings for solid gate dielectrics were cha
Hydrolysis-condensation of bis(triprop-1-ynylstannyl)butylene led to nanostructured bridged polystannoxane films yielding tin dioxide thin layers upon UV-treatment or annealing in air. According to Fourier transform infrared (FTIR) spectroscopy, cont
This review deals with the correlation between morphology, structure and performance of organic electronic devices including thin film transistors and solar cells. In particular, we report on solution processed devices going into the role of the 3D s
Among the metal oxide semiconductors, ZnO has been widely investigated as a channel material in thin-film transistors (TFTs) due to its excellent electrical properties, optical transparency and simple fabrication via solution-processed techniques. He
Solution-processed metal oxide thin-film transistors (TFTs) operating in enhancement mode are promising for the next-generation flat panel displays. In this work, we report high-mobility TFTs based on SnO2 active layer derived from a soluble tin(II)
Lithium (Li)-assisted indium oxide (In2O3) thin films with ordered structures were prepared on solution-processed zirconium oxide (ZrO2) gate dielectrics by spin-casting and thermally annealing hydrated indium nitrate solutions with different Li nitr
A common feature of the inorganic thin films including Cu(In,Ga)(S,Se)2 fabricated by nonvacuum solution-based approaches is the doubled-layered structure, with a top dense inorganic film and a bottom carbon-containing residual layer. Although the la
Considering that topological insulator (TI) ultrathin films (UTFs) provide an ideal platform for the transport measurement of topologically protected surface states, we have investigated the transport properties of the three-dimensional (3D) TI UTFs
Local piezoresponse and piezoelectric output voltage were evaluated on ZnO thin films deposited by radio-frequency magnetron sputtering on hard Si/Ti/Au and flexible Cu-coated polyimide substrates. Three different thicknesses of ZnO films were studie